title: Polymerization shrinkage and depth of cure of bulk fill flowable composite resins.
abstract: OBJECTIVE
  To evaluate polymerization shrinkage and depth of cure of two bulk fill flowable composites, one nanohybrid composite modified to a flowable consistency, and one standard flowable composite, comparing the scraping method to the Knoop hardness test.
  
  
  METHODS
  Two bulk fill flowable composites, SureFil SDR flow (SSF) (Dentsply) and Venus Bulk Fill (VBF) (Heraeus Kulzer), one standard flowable, Filtek Supreme Ultra Flowable (FSUF) (3M/ESPE) (control), and one regular bulk composite that can be made flowable, SonicFill (SF) (Kerr), were used in this study. For polymerization shrinkage (PS), ten 2-mm samples were made for each composite and cured for 20 seconds and shrinkage was measured with a Kaman linometer. For hardness, ten specimens of each composite were made in a 10 × 10-mm mold and cured for 20 seconds; the bottom surface was scraped according to ISO 4049 specification, and the remaining thickness was measured with a micrometer. Hardness samples were prepared at 2-, 3-, 4-, and 5-mm thick ×14-mm diameter, cured for 20 seconds, and polished. After 24 hours of dry storage, a Knoop indenter was applied at 100 g load for 11 seconds. Three readings were made on the top and bottom of each specimen and averaged for each surface to calculate a Knoop hardness value and a bottom/top hardness ratio. One-way analysis of variance and Tukey tests were used to determine significant differences between thicknesses and between test methods for each material.
  
  
  RESULTS
  PS values were 3.43 ± 0.51%, 3.57 ± 0.63%, 4.4 ± 0.79%, and 1.76 ± 0.53% for FSUF, SSF, VBF, and SF, respectively. VBF showed significantly greater shrinkage (4.4 ± 0.79%), followed by FSUF (3.43 ± 0.51%) and SSF (3.57 ± 0.63%), which were similar, and SF (1.76 ± 0.53%), which had significantly less shrinkage (p<0.05). Values for the scraping method for depth of cure were significantly greater for SSF and VBF (>5.0 mm), followed by SF (3.46 ± 0.16 mm) and FSU (2.98 ± 0.22 mm). Knoop top hardness values (KHN) were: VBF 21.55 ± 2.39, FSUF 44.62 ± 1.93, SSF 29.17 ± 0.76, and SF 72.56 ± 2.4 at 2 mm and were not significantly different at 3-, 4-, and 5-mm thick within each material. Ratios for bottom/top values (depth of cure) for 2, 3, 4, and 5 mm were: VBF 0.80 ± 0.1, 0.78 ± 0.03, 0.67 ± 0.10, and 0.59 ± 0.07, respectively; SSF 0.74 ± 0.08, 0.72 ± 0.08, 0.69 ± 0.18, and 0.62 ± 0.08, respectively; SF 0.82 ± 0.05, 0.68 ± 0.05, 0.47 ± 0.04, and 0.21 ± 0.02, respectively; and FSUF 0.56 ± 0.08 at 2 mm and 0.40 ± 0.08 at 3 mm. The bottom/top ratio was .80 or less at all depths and decreased below 0.70 at 4-mm depth for VBF and SSF, at 3 mm for SF and at 2 mm for FSUF.
authors.forename: D
authors.initials: D
authors.lastname: Garcia
authors.forename: P
authors.initials: P
authors.lastname: Yaman
authors.forename: J
authors.initials: J
authors.lastname: Dennison
authors.forename: Gf
authors.initials: G
authors.lastname: Neiva
mesh_terms: D003188:Composite Resins; D006245:Hardness Tests; D058105:Polymerization; D013499:Surface Properties
chemical_list: D003188:Composite Resins